advertisement

AN ABSTRACT OF THE THESIS OF Na Li for the degree of Master of Science in Mechanical Engineering presented on April 13, 2001. Title: Metallurgy and Superconductivity of Niobium-Titanium-Tantalum Ternary Alloy System. Redacted for Privacy Abstract approved: William H. Warnes The metallurgy and superconductivity of the Nb-Ti-Ta ternary alloy system were studied. The Nb-Ti, and Ta-Ti binary samples, and Nb-Ti-Ta ternary samples were precipitation heat treated under different schedules. After the precipitating heat treatment, the samples were characterized by X-Ray Diffraction (XRD) techniques. Equilibrium binary and ternary phase diagrams based on the different alloy compositions and heat treatment temperatures were developed. The Ta-Ti binary phase diagram is very close to the ASM standard phase diagram. The 3-phase boundary of Nb-Ti binary phase diagram developed here is at a higher temperature relative to the ASM standard one. A working ternary equilibrium phase diagram for the Nb-Ti-Ta system has been developed that is based on the experimental measurements and quantitative thermodynamic calculations. Measurements of superconducting critical temperature, Tc, show a good agreement with previous measurements of Tc in the ternary alloys. © Copyright by Na Li April 13, 2001 All Rights Reserved METALLURGY AND SUPERCONDUCTIVITY OF NIOBIUMTITANIUM-TANTALUM TERNARY ALLOY SYSTEMS by Na Li A Thesis submitted to Oregon State University in partial fulfillment of the requirements for the degree of Master of Science Presented April 13, 2001 Commencement June 2002 Master of Science thesis of Na Li presented on April 13, 2001 Approved: Redacted for Privacy Maj or Professor, representing Mechanical Engineering Redacted for Privacy Head of Department of Mechanical Engineering Redacted for Privacy Dean of I understand that my thesis will become part of the permanent collection of Oregon State University libraries. My signature below authorizes release of my thesis to any reader upon request. Redacted for Privacy ACKNOWLEDGMENTS I would like to acknowledge the constant support and encouragement received over the years from my professor, William H. Warnes. Anytime I struggled with experimental results, felt disappointed or need assistant, he was always willing to give advices and render aid. In particular, I wish to thank Alexander Yokochi from Chemistry Department for his guidance with running x-ray analysis and Roger Neilson from College of Oceanography for performing with electron microprobe analysis. The financial support of the Fermi National Acceleration Laboratory is gratefully acknowledged. Without their support, this project couldn't be fulfilled. TABLE OF CONTENTS INTRODUCTION AND BACKGROUND Introduction and background ................................................................................ 1 Literaturereview ................................................................................................... 2 Binary phase diagrams .............................................................................. 2 Contamination Effect on Binary Phase Diagrams .................................... 5 Ternary phase diagrams ............................................................................ 5. Superconducting properties ................................................................................... 7 Critical temperature ................................................................................... 7 Uppercritical field .................................................................................... 8 Critical current density .............................................................................. 9 Conclusions ............................................................................................. 14 EXPERIMENTAL PROCEDURES ............................................................................... 16 Samplesources .................................................................................................... 16 Electron microprobe analysis .............................................................................. 16 Annealingconditions ........................................................................................... 17 X-ray-diffraction analysis ................................................................................... 18 XRDpeak fitting routine ......................................................................... 18 XRD data analysis routine ....................................................................... 19 Critical temperature measurement .......................................................... 20 RESULTS AND DISCUSSION ..................................................................................... 22 EMPA results on sample homogeneity .............................................................. 22 Binarysystems .................................................................................................... 23 X-ray diffraction results .......................................................................... Phase diagram calculations by regular solution model ........................... 28 Contaminationeffect ............................................................................... 33 Kinetics of and x transformations ........................................................ 33 Ternary alloy systems .......................................................................................... 36 f3 Ternary samples and adopted model ....................................................... 36 Ternary alloy phase diagrams .................................................................. 37 TABLE OF CONTENTS (CONTINUED) .37 Thermo-calculation phase diagrams X-ray diffraction results .......................................................................... 37 Diffusion behavior of ternary alloys ................................................................... 40 Critical temperature for binary and ternary alloy systems .................................. 42 Conclusions ......................................................................................................... BIBLIOGRAPHY ................................................................... 45 APPENDICES ......................................................................... 50 Appendix I. X-ray analysis routine ............................. 51 Appendix H. Regular solution model of binary and te nary phase equilibria ..... 55 Appendix III. Critical temperature measurement ........ 60 Appendix IV. Critical temperature data ...................... 62 LIST OF FIGURES Figure Page 1. The binary Nb-Ti alloy system at low temperature ................................................ 4 2. The binary Ta-Ti alloy system at low temperature ............................................... 4 3. The type B ternary diagram from reference ........................................................... 6 4. The schematic of critical temperature measurement ............................................ 21 5. Ta-Ti x-ray diffraction patterns for different temperature heat treatment 6. Typical Nb-Ti samples XRD pattern under different heat treatment temperatures. ......... 24 ................................................................................................................ 25 7. The binary Ta-Ti alloy system at low temperature .............................................. 31 8. The binary Nb-Ti alloy system at low temperature .............................................. 31 9. Semilog plot of the diffucivity as a function of the inverse of the temperature for Ta-Ti binary alloy ................................................................................................. 35 10. Comparison of interdiffusion coefficients of Nb-Ti and Ta-Ti binary systems...35 11. Type B ternary phase diagram and investigated ternary samples ........................ 38 12. Experimental data from precipitating heat treatment at different temperatures in Nb-Ti-Ta ternary alloy system .............................................................................. 39 13. Extrapolated ternary equilibrium phase diagram for the Nb-Ti-Ta system ......... 40 14. Ternary diffusivity-Lines of constant diffusivity plotted on the Nb-Ti-Ta ternary phase diagram at temperature 400°C ...................................................................41 15. Ternary diffusivity-Lines of constant diffusivity plotted on the Nb-Ti-Ta ternary phase diagram at temperature 500°C .................................................................... 41 16. Ternary diffusivity-Lines of constant diffusivity plotted on the Nb-Ti-Ta ternary phase diagram at temperature at 600°C ................................................................42 17. Critical temperature as a function of alloy compositions..................................... 44 LIST OF TABLES Table 1. Lattice parameters of Nb, Ti, and Ta elements ........................................................ 2 2. 3. Critical temperatures of binaries, ternaries, and quarternaries under certain heat treatment conditions ................................................................................................. 7 Upper critical fields of binaries, ternaries, and quaternaries from literature .......... 10 4. GLAG theory related parameters determined for binaries and ternaries ............... 11 5. 6. a-Ti precipitates at different heat treatments for ternary similarly processed binary alloys................................................................................................................. 13 Jc vs. magnetic field at different heat treatment at 4.2 K ....................................... 14 7. The sources of samples and heat treatment conditions .......................................... 17 8. Chemical analysis of ternary samples using electron microprobe analysis ........... 22 9a. Ta-Ti x-ray diffraction data .................................................................................... 26 9b. Nb-Ti x-ray diffraction data ................................................................................... 27 10. Regular solution parameters for Ti-based stable equilibria .................................... 29 1 la. Ta-Ti binary phase boundary .................................................................................. 29 1 lb. Nb-Ti binary phase boundary ................................................................................. 30 12a. Nb-Ti-Ta ternary n-phase boundary-XRD ............................................................. 38 12b. Nb-Ti-Ta ternary n-phase- boundary-Calculation ................................................. 39 LIST OF APPENDIX FIGURES Figure ig Al. The atomic scattering factors .............................................................................. 54 A2. Free energy representation of formation of ternary phase equilibria .................. 57 A3. Critical temperature measurements ..................................................................... 61 A4. Critical temperature verse the heat treatment ...................................................... 62 LIST OF APPENDIX TABLES Table Page Al. Multiplicity factors A2. The notation used in NbTiTa ternary system ..................................................... 56 A3. Critical temperatures at different aging times and aging temperatures .............. 67 .53 LIST OF ABBREVIATIONS, SYMBOLS and NOTATIONS A Amper a Hexagonal crystal lattice parameter a0 Cubic crystal lattice paramater Ar Argon at% Atomic percent Avg. Average BCC Body centered cubic (crystal lattice) c Hexagonal crystal lattice parameter °C Degree Celsius CSA Cross section area CW Cold work d Diameter D Interdiffusion coefficient D0 Frequency factor dg Degree angle EMPA Electron microprobe analysis GLAG Ginzburg, Landau, Abrikosov, and Gor'kov H Magnetic field Hc2 Upper critical Field HCP Hexagonal close packed (crystal lattice) H0 Upper critical field at absolute zero h Hours Jc Critical current density K Kelvin Nb Niobium NHT No heat treatment NT Niobium-Titanium alloy pet Percent of titanium ppt Precipitate R Gas constant s Second T Temperature Ta Tantalum Tc Critical temperature TEM Transmission electronic microscope Ti Titanium TT Tantalum-Titanium alloy wt% Weight percent XRD X-ray diffraction V% Volume fraction Strain Electronic specific heat coefficient Jio Permeability of free space = 4itx 10 p Normal state resistivity In this thesis, all alloys are in weight percentage except special noticed. DEDICATION Dedicated to Mom and Dad. METALLURGY AND SUPERCONDUCTIVITY OF NIOBIUMTITANIUM-TANTALUM TERNARY ALLOY SYSTEMS INTRODUCTION AND BACKGROUND Introduction: High Energy Physics has long supported the study of superconductivity, especially the high-field, high current density superconductors. The reason for this has been the attractiveness of superconducting materials for use in accelerator magnets for beam steering, control and focussing. Of the low temperature metallic superconductors one potential candidate for fabricating high field electromagnets is the Nb-Ti-Ta ternary system. The ternary alloys show higher critical magnetic fields than the Nb-Ti binaries as the temperature is decreased. The attractions of these materials for magnet construction are its ductility and ease of handling relative to A- 15 intermetallic or ceramic high temperature superconductor (HTS) competitors. There are many questions about the potential for the ternary alloys, principally relating to fabricability and optimum critical current density at high fields. Recent work, funded at our laboratory by Fermi National Accelerator Laboratory, has used existing literature information to develop an understanding of the equilibrium ternary phase diagram of the Nb-Ti-Ta system, and has provided insight as to the alloy compositions and heat treatments that are likely to lead to higher performance in this system 1 2] The previous understanding of the metallurgy of this system has been limited by a lack of information in the literature about the equilibrium properties of the alloys of interest, as well as by a dearth of studies on the precipitation behavior. Both of these limitations can be overcome by additional experimental work on the superconducting alloys with the best potential for high critical field and current density. Literature Review: Binary Phase Diagrams The atomic v&lume difference among Nb, Ti, and Ta is small. According to JCPDS data, the atomic volume difference between Nb and Ta is 0.02 pct and 2.9 pct between Nb/Ta and Ti. A 2% volume difference 41 a 1.3 % diameter difference151 between Nb and Ti are also reported ( Table 1). Table 1 Lattice parameters of Nb, Ti, Ta elements (A). a is the bcc- phase parameters, and aa is the hcp a-phase parameter. value for pure elements Nb Ta a a a/aa 3.3030 3.3058 -/2.9505 4.6826 3.3067 3.2980 3.3066/2.9512 - -/2.9503 4.6845 Ti C 113] [6] d (lattice adjacent plane spacing) [6] 1.43 4.683 1 1.45 1.43 The very small atomic size difference between Nb and Ta results in an isomorphous system of continuous series of solid solutions. In NbTi and TaTi binary systems, the BCC elements form a partial miscibility gap with a -Ti (HCP) in the presence of a stable 13 phase solid solution (BCC). The major difference between the NbTi and TaTi binary phase diagrams is that the 13-phase boundary in TaTi is at lower Ti concentration than that in the NbTi binary system. In other words, the 13phase boundary in TaTi binaries is located at higher temperatures when compared to the same alloy composition in Nb-Ti. All three binary systems have been studied extensively in ASM [7i8j The phase diagram of NbTa shows a complete miscibility of Ta and Nb in the solid. 3 At present, although the author admits that "there is a fundamental difficulty in determining the thesis transus in this alloy (20 at % to 70 at % Nb) system", Moffat's Ph.D. been considered as the most systematic work done on the NbTi binary phase diagram. His results were based mainly on his predictions and the experimental data at high temperatures from others work [6-I2j No one, however, has ever done experiments below 600°C because the diffusion rate is believed very slow at low temperature and it takes a long time to reach the equilibrium state. There are two sets of data representing the Nb-Ti phase diagram, as shown in Figure 1. One is from Kaufman's prediction data obtained from Hansen [8j 1ifl This calculation is very close to the experimental Hansen believed that his results represent the conditions close to the equilibrium. Another set of data is from Murray's prediction '°', as well Brown's experimental work [9] Although Murray's work is part of the ASM 8j binary phase diagram, Moffat believed that "the resultant negative 13 phase interaction parameter Murray initialized was acknowledged as being physically unreasonable in this system". The data in references 19-25 in Figure 1 are experimental measurements of microstructure that are interpreted here with the lever rule to find the 13-phase boundary. All literature data about Ta-Ti binary phase diagrams system is shown in Figure 2. Summer's 11516[ show a higher tantalum content 13-phase boundary than the ASM published data at all temperatures. He didn't do the experiment below 700°C. However, his extrapolated data at 650°C and 600°C are all higher than that of other's work. Maykuth' s results [hlj are closer to the published phase boundary, but still higher than all other works except Summer's. Chernov, et al [2 is very close to the ASM data. The solubility of Nb and Ta in a -Ti increases as the temperature is lowered. Nb is less soluble in a -Ti than Ta is. In the 13-phase, BCC elements lower the transition point of titanium, thus stabilizing the 13-phase. So, we call them 13-phase stabilizers. Of four elements with partial miscibility with a -Ti alloys (Nb, V, Mo, Ta), Ta has the widest a--13 two-phase region. Therefore, Ta is the weakest 13-phase stabilizer. Nb-Ti Binary Alloy Phase Diagrams Ref 18 850 750 650 550 0. 350 0 20 40 60 80 Weight percent of niobium (wt.%) Figure 1. The binary Nb-Ti alloy system at low temperatures. The solid lines indicate the standard binary phase diagramUS]. The symbols show the experimental results from various references (see legend). Ta-Ti Binary Phase Diagrams 900 cRef.18 850 E 0 20 40 60 80 100 Weight percent of tantalum (wt. %) Figure 2. The binary Ta-Ti alloy system at low temperatures. The solid lines indicate the standard binary phase am1181 The symbols show the experimental results from various references (see legend). 5 Contamination Effect on Binary Phase Diagrams When heat-treated at high temperature, the samples are very easily contaminated with oxygen. Contamination may cause the lattice to distort and affect the position of the phase boundary. These interstitial atoms obtain high thermal energy when they are heated up. It has been shown theoretically that carbon, nitrogen, and oxygen in interstitial solution lower the free energy of the a phase relative to thesis as well 17j 13 phase. The predicted results are shown in Moffat To demonstrate this effect, Hansen, et al ' prepared two different Ti-Mo samples (representing high and low levels of impurities) and found out that the 13-phase boundary in high impurity alloys is about 20% higher in temperature than that in low impurity ones. Ternary Phase Diagrams There is a very limited amount of work done on the Nb-Ti-Ta ternary composition temperature phase diagrams. In Warnes et al. work 1], they successfully established ternary diagrams combining temperature and composition information into one plot, as shown in Figure 3. By searching and analyzing the existing literature data on Nb-Ti-Ta ternary alloys and corresponding binary systems, a reasonable prediction of the minimum 13-phase boundary position and optimization for the H2 and J were proposed They believe that most samples studied in the past were either on the lower Ta composition side, or at the top of, the H2 peak. If samples are at a low Ta content, one can never obtain the H, peak from them because they are far from the H2 peak and the precipitation tie line will never pass through the H2 peak region at all. On the other hand, if samples are at the top of or a little bit off the H2 peak, the precipitating heat treatment will easily overshoot and miss the H2 peak due to the faster kinetics of Ta-ternary alloys. The other problem suggested by the authors is that the precipitating temperatures have been too low to optimize H2. As shown in Figure 3, even at 420 °C heat treatment, the predicted 13-phase boundary is still on the lower side of the H2 peak. Nb 380C -15.4T 1 5T 14.6T 1 4T -131 1 2T ref samples 4200 $00 Ta Ti -I '1 U, - U, U, U, U, Figure 3. The type B ternary diagram from reference The H, contour plot at 2.0K, and the 380 °C and 420°C 13-phase boundary predicted are also plotted here. The dots are ternary samples investigated up to now. As far as we know ', 420°C is the highest precipitating heat treatment temperature that has been attempted for optimizing high H2 or J in Nb-Ti-Ta ternary system. The suggested solution for this is to use higher precipitating temperature to heat-treat the samples of the right composition. This is also the guideline for us to deal with our samples later on. We haven't seen any other reports in the literatures on Nb-Ti-Ta ternary phase diagrams. Superconducting Properties Critical Temperature (Tc) Generally, the critical temperature is considered to decrease by additions of Ta, Hf, and Zr to the binary system with Nb due to the lower critical temperature of these elements compared to Nb. The critical temperatures for pure Nb, Ta, Hf, Zr are 9.5 K, 4.4 K, 0.12 7 K, and 0.55K respectively. However, for up to 6 at % Ta the decrease in Tc is very small ]27] Tc of the alloys is affected by heat treatment. Both aging time and aging temperature influence Tc. In the study of the tern aries, Wada et al found that in the NbTiHf ternary alloy, 3 at % Hf increases Tc at all aging temperatures 1281 The addition of Hf (Ti 40 at % Nb 3 at % Hf) causes a Tc increase of about 0.3 K over Ti-40 at % Nb. More than 6 at % Hf additions, decrease Tc when the aging temperature is below 600°C. With an aging temperature of 800°C, addition of Hf tends to increase the critical temperature. X-ray analysis revealed that aging at 800°C caused significant precipitation of a-phase in high Hf alloys. Table 2. Critical temperature (K) of binaries, ternaries and quaternaries under certain heat treatment conditions. Alloys (wt. %) Tc TERNARIES 9.l(extrusion + 80% cold drawing) 9.1 (extrusion + 80% cold drawing) 8.7 (homogenized at 1300°C/8h) 8.99 (homogenized at 1300°C18h) 8.2 8.85 9.45 (450°C/60h) 9.4 (375°C140h) 8.33 7.17 9.5 6.5, 8.4 (380°C/800h) BINARIES 7.3 (380°C/80h) 8.52 references Nb46.5Ti 8.9,9.42 (372°C/40h) Nb18.lTi 10.1 30, 19 30 NbTiTa2O NbTiTal2 NbTiTa2O NbTiTal2 Nb25Ta 45Ti Nbl5Ta44Ti Nb4OTil8Ta Nb4lTi28Ta Ti38Nbl6Ta Til6Nb44.8Ta Nb62.5Ti7.2lHf Nb64.5TilZr Nb65Ti Ti5ONb 29 29 29 29 30 30 19 19 27 27 28 20 20 27 The critical temperature increases with the aging time of NbTiZr [201 The critical temperature of Zr specimens aged at 380°C for 800 hours increases from 6.5 K (see Table 2) up to values of about 8.4K. Panek attributes the enhancement of Tc with increasing aging time to the Nb enrichment of the matrix that accompanies the ct-Ti precipitation, as determined using TEM. The critical temperature of Hf ternary specimens aged above 600 °C can be increased from 8.0K-8.3 K up to 9K [20[ Aging time or temperature can have a significant effect on critical temperature. The Tc of a variety of NbTi ternary and binary alloys under a range of process conditions is given in Table 2. Upper Critical Field (Ha) The upper critical field of binary NbTi is normally suppressed by spin-orbit-coupling. Alloying with an element of high atomic number, such as Ta, Hf, or Zr can suppress the paramagnetic limitation, and reduce spin-orbit-coupling through spin-orbit-scattering. There should be a stronger enhancement of H7 at lower temperature because at lower temperature, the paramagnetic limitation becomes stronger. H2 is temperature dependent as, H. [1 -(TIT)2]. At 4.2K, the enhancement of H C2 in the ternaries is slight, with small increases of 0.15 tesla 1201 0.2 tesla 131j and 0.3 tesla reported. This is shown in Table 3. At 4.2K, no significant difference is seen between the H2 of the binaries and Ta-ternaries. The highest H2 (13.6 Tesla) at 4.2K is observed in Nb22Ti22Zr. In the NbTiTa case, replacing Nb with Ta enhances H2 (4.2 K) up to 10 to l5Ta depending on Ti concentration 132[ At around 2.0 K, Hc2 can be raised from 14.1 tesla for the best binary (Nb 46.5Ti) to 15.5 tesla (Nb 42Ti l9Ta) Nb4lTi28Ta) Hc2 [20. 31, 331 [31[, and 15.4 tesla (Nb43Ti 25Ta, for the ternary alloys. is also a function of normal state resistivity (pa), electronic specific heat coefficient (y), and critical temperature (Tc). At 0 K, the relation is given by GLAG theory 311 as: ;sJ = 3.1 xl O3'yp,T (tesla) Equation 1 It is reported [3] that when replacing Nb by Ta, Tc decreases slowly, and y, pn do not change. This therefore results in a gradual decrease in H0. By replacing Ti by Hf, a rapid reduction of Tc and y results in a decrease of H. Suenaga reported alloys in the 64 at % Ti series, a decreased Tc and pn 301 that for Nb-rich due to the replacement of Ta for Nb caused a decrease in critical field. From Table 4, it can be seen that adding a third element produces higher normal state resistivity and lower critical temperature (except for 2.5 Hf-ternary in which Hf-concentration is too low to influence the overall critical temperature) compared to the binaries. The concentration of Ta does not strongly influence the p,,, while in Hf-ternaries, p increased obviously with the Hf concentration. According to Hawksworth 3!] the H0 of the ternaries is equal to or less than the binaries, except for the case of 5 at % Ta that increased the H, (see Table 4). Critical Current Density (Jc) Adding the third component increases the diffusion rates of Ti, and therefore accelerates the precipitation kinetics of a-Ti [20) So, generally, NbTiTa ternary alloys produce 10% more volume fraction of precipitates for the same heat treatment schedules than the binaries. However, the precipitate size in the ternary is larger than that in the binary. Taillard 2fl found growth of alpha precipitates on subband cell walls after heat treatment. In the ternary alloys, however, a relatively low concentration of a third element can sup- press during cooling and accelerates precipitation of the stable a-phase. Also, a large prestrain (6.4-7) can suppress the o-phase in both binary and ternary alloys. The co-phase is a metastable phase which growsisothermally. Larbalestier stated that Zr additions form precipitates more easily due to the larger atomic size of Zr. Precipitation of a-Ti containing Zr may therefore form more rapidly than in binary alloys. However, replacing Ti by Zr may result in a reduction in the quality of a-Ti precipitate for flux pinning 123] 10 Table 3. Upper critical fields (Tesla) of binaries, ternaries and quaternaries from literature. Alloy (wt %) 4.2K 2.0 K References TERNARIES Nb44.8Ti-12.3Ta 10.4 (er=4) 13.3-13.4 (2.2K); 14.1,14.3 (1.85K) 29,34 Nb42.6Ti20.4Ta 10.3 (c=4) 13.4-13.8 (2.2K); 14.3, 14.5(1.85K) 29, 34 Nb44Ti25Ta 10.4 14.4 35 Nb45Ti25Ta 10.9 14.8 32 Nb44Til5Ta 11.6 15 32 Nb45.7Ti13.3Ta 11.6 15 31 Nb43Ti25Ta 11.6 15.4 31 Nb40.5Ti35.3lTa 11.1 15.3 31 Nb33.4Ti44.5Ta 10.9 15.2 31 Nb42Til9Ta 15.5 19 Nb4lTil3Hf 14.5 19 Nb44.7Ti6.7Hf 11.3 14.35 31 Nb40.9Ti12.7Hf 11 14.5 31 Nb34Ti23Hf 10.4 14.2 31 Nb22Ti22Zr 13.6 31 NbTiI5Ta* 14.3 (1.8K) 22 NbTi25Ta 14.7 (1.9K) 22 Nb4OTil8Ta 11.03, 11.7 13.53, 15.2 20,33 Nb4lTi28Ta 10.25, 11.3 14, 15.4 20,33 14.3 34 Nb43.9Til4Ta QUARTERNARIES Nb39Ti24Ta6Zr 13.1 Nb38Ti26Ta6Hf 11.3 31 15.3 31 BINARIES Nb46.5Ti Nb9.82at.%Ti 10.53, 11.3, (--), 10.3, 11.3 Nb49Ti 12.2 Nb38Ti 11.4 Nb5OTi Nb48Ti 11,5 (--) 13.28, 14.1,14.2 20,33,36 13.7, 14.1, 14.2 35, 32, 19 31 31 12.7 (1.8K) 22 14.25 31 11 Table 4. GLAG theory related parameters determined for binaries and ternaries Alloys (at%) p (G.m) Nb64.2Ti 6.5 Nb65Ti5Ta Tc (K) H0 0.92 9 16.5 6.8 0.9 8.9 16.7 Nb65TilOTa 6.7 0.93 8.6 16.5 Nb65Til5Ta 6.9 0.94 8.15 16.2 Nb65Ti2OTa 6.7 0.92 8.1 16.5 Nb62.5Ti2.5Hf 6.8 0.87 9 16.4 Nb6OTi5Hf 6.9 0.91 8.5 16.4 Nb55TilOHf 7.25 0.83 8.35 15.45 Y( mmK 2) [31] and thus the magnitude of Jc. Accelerated a-Ti precipitation is also found in the Taternaries. This is believed to be due to the fact that the Ta is a weaker 3-phase stabilizer than Nb L29 In the binary system, Jc increases proportionally to the cL-phase volume fraction. Lee expressed the Jc as a V% of a-Ti precipitate as: Jc= 120 V%+675 (5 tesla) and Jc 41 V% +470 (8 tesla). However, in NbTiTa, NbTiHf, and NbTiZr ternary systems, although a higher a-precipitate volume fraction than binary is observed, Jc is in general lower than that in binary, as shown in Table 5. Although the ternary has a higher volume fraction of alpha precipitates, it also has a larger precipitate size. Jc relates both to the alpha precipitate size and the volume fraction. Jc is dependent on the final strain after last heat treatment. Addition of Zr produces a significant (1) shift of strain at peak Jc to lower strain 1231 Also, the Jc peak is brought down to lower value. However, some studies have shown that the Jc of the ternary alloys is somewhat independent of final strain [233839] One might expect that the lower strain to peak Jc in the ternaries to coincide with a relatively smaller precipitate. However, this is 12 not always the case. From Table 5, it is hard to get a conclusion that Jc increases with either precipitate size or mean cross section area. An aggressive heat treatment was suggested 24 improve the precipitate volume fraction in the ternaries. Jc increases with the heat treatment temperature until it reaches the peak at 475°C. Extending the treatment temperature or time can increase the precipitation, as shown in Table 5. However, Shimada shows in his work that there was no benefit or even worse from prolonged heat treatment time for high field (7 tesla) Jc. Another way to increase the precipitation rate is to replace Nb with Zr rather than with Ti [2324] The later approach may deteriorate Hc2 and thus high field properties. High field Jc near Hc2 is well known to be less sensitive to heat treatment and microstructure than at lower field 13'l As shown in Table 6, heat treatment is effective in improving low field Jc. At high magnetic fields, the dependence of Jc on H is large and then the upper critical field becomes the dominant factor in determining Jc. Of ternary alloys, Nb 65 at % Ti 10-12.5 at % Ta is about the best for high field use because its upper critical field is the maximum (Table 3). There is a report [38391 that at low magnetic field (5 Tesla and 7Tesla), lower Ta ternary alloy (Nb44Ti8Ta) has higher critical current density than higher Ta ternary alloy (Nb43Ti25Ta). However, at high magnetic fields (12 Tesla), higher Ta ternary alloys, such as 25Ta, showed a better performance than the 8Ta. 13 Table 5. u-precipitate at different heat treatments for ternary and similarly processed binary alloys. Alloy (wt%) 45Til5Ta/Nb47Ti 45Til5Ta/Nb47Ti V% of a-Ti Heat Treatment a 45Ti1 5Ta/Nb47Ti 45Til5Ta/Nb47Ti 45Ti25Ta/Nb46.5Ti 45Ti25Ta/Nb46.5Ti 45Ti25Ta/Nb46.5Ti 44Til5Ta/Nb46.5Ti 18/17 2X80h/380°C 20.1/16.5 2X80hJ420°C 3X40h/380°C 4X40hI380°C 24-25/22 28/24 25.2/17.8 23.3/ 24.8/18.6 2325/ 927/1174 35 35 35 35 123/107 2000/2800 290/950 40 112 40 127/114 203/140 163/194 46/181 65/82 2000/3000 290/950 2000/3000 240/950 114-118 44TiI5Ta/Nb465Tj 46.lTil.9Zr/Nb46.5Ti 27/24 48.9Ti3.8ZrfNbS3Tj 4OTil8Ta/Nb46.5T 16/28 13.7-14.5 4X40/375°C 4lTi28Ta/Nb46.5Ti Nb45Til5Ta Nb45Til5Ta Nb45Til5Ta 16.4/ 25/22 28/24 3X40W380° C 4X40h/380° C 18/17 Nb44.4Ti l5Ta 12.5 2X80h/380°C 6h!405°C+ 20h/420°C+ Nb44.4Til5Ta 14 Nb44.4Til5Ta 16.25 Nb44.4TiI5Ta 21 Nb44.4TII5Ta 21 14/21 Jc (A/mm2) Jc (A/mm2) references (5Ts, 4.2K) (8Ts, 4.2K) 1.5h/800° C 40h/375°C CW 3x80/420° C 5x80/420° C 3x80/420° C 3x80/420°C 25/21 Mean CSA Avg. a-Ti d (nm) (nm2) 107 32300/15500 20870/29660 5095/41882 3035/3200 1350/750 4846/12327 2800/3200 1100/750 2265-2497 1221 1840 812 24x2.7 2370/2580 910/1220 24x2.7 2810/3050 900/1220 33x3.8 2280/2570 910/1200 40 41 41 23 23 20 20 21 21 21 1700 825 42,43,44 2250 900 42,43,44 2x3h/300° C+ 6h/405°C 2300 950 42,43,44 2x3h/300°C 80h/420°C 2700 1050 42.43,44 3h1300°C6h/405° C+ 2800 42,43,44 Nb4lTi28Ta 3x40h/450° C 2647 843 25 Nb44Til7Ta 3x40h/450°C 2671 992 25 NB46T1I2Ta 3x80b/450° C 3075 959 25 Nb44Ti I 7Ta(multi-) 3x80h/375°C 2534 848 25 Nb44Ti l7Ta(multj-) 4x80h/375° C 2724 785 25 Nb44Til7'fa(mu}tj-) 20h/450° C+2x80h1375° C C,8Ts, 2637 786 25 2550 821 24 4x48h/380°C 2x6h/350°C-i-1x40hJ380°C 5x12W350°C 5x12h/380°C 4x48h/380°C 2x6h1350aC+1x40h/3800C 2170 1970 800 780 750-800 43.34 43,34 5x12h/350°C 1650 1850 2500 Nb41 Ti28Ta Nb43Ti2OTa Nb43Ti2OTa Nb43Ti2OTa Nb43Ti2OTa Nb45Til2Ta Nb45Til2Ta Nb45Til2Ta Nb45Til2Ta Nb44TiI4Ta Nb44Tjl4Ta Nb47Ti Nb44Til4Ta a 5x12b1380°C 5x12h/400°C 5x12h/350aC 5x12h/350°C ternary/binary number of heat treatment x hours! temperature (°C) 1200 1800 2250 2000 1990 1280 750800 825 900 850 850 1150 1000 700 34 34 34 34 34 34 34 34 34 34 14 Table 6. Jc (A/mm2) vs. magnetic field at different heat treatment at 4.2K291. Field (Tesla) 45 h 85 h 200 h 5 1850 2245 2200 6 1490 1650 1550 7 1125 1125 1000 8 650 625 490 Conclusions: From studies done and reported in the literature, the following conclusions are drawn: 1. Uncertainty is still exists not only in Ta-Ti, but also in the Nb-Ti binary phase diagram. 2. The Nb-Ti-Ta ternary temperature-composition phase diagram is unknown. Warnes gives us a pretty good outline to start with. 3. At 4.2 K, even the best ternary alloys showed no significant improvement in either critical field or critical current density. At low temperature, the Ta-ternary can perform much better than the binary does. 4. NbTiZr or NbTiHf conductor did not perform as well as NbTiTa in high field 135] [23], When used in high field, NbTiTa has been shown to have significantly higher current density and critical field than NbTiZr or NbTiHf. 5. Cold work after the heat treatment is found to be more effective in increasing Jc in high fields than in low field for NbTiHf. Cold work plays a critical role in high field Jc performance (8 Tesla). 6. Critical current density depends strongly on the heat treatment. However, the size of cx-precipitate does not produce a consistent effect on Jc. In general, it is believed that a smaller a-precipitate size is a good pinning center and therefore results in a higher Jc. 15 7. Homogeneous NbTiTa yields higher Jc than inhomogeneous composite because homogeneous starting material produces smaller more uniform precipitation, and thus raises Jc. 8. Large prestrains of 6.4-7 are required to suppress the deleterious o-phase in the Ta-ternaries. 9. Binary alloys have a lower volume fraction of alpha precipitate, but higher Jc than similarly processed ternaries. EXPERIMENTAL PROCEDURES In order to better understand the equilibrium ternary phase diagram, several experiments were undertaken: EMPA, XRD, and Tc measurement. The as-received samples were basically divided into two sets. One set of these as-received samples was examined under electron microprobe analysis to determine the impurities of the sample. Another set of asreceived samples was heat-treated under different schedules (as shown in Table 7), and then XRD was done to identify the phase composition of these samples. Finally, after the XRD test, the critical temperature of the second set of samples was measured. The details are described below. Source of Samples: Binary samples were obtained from Oremet-Wah Chang, Albany, Oregon. Ternary samples were obtained from Intermagnetics General Corporation, Waterbury, Connecticut. Bulk samples were cleaned using acetone and methanol. Multifilamentary samples were put into acid to remove the copper, and then cleaned. Electron Microprobe Analysis (Impurity-Analysis): Electron microprobe analysis was carried out on four out of six ternary samples in the asreceived state to determine their composition and the homogeneity. Nb24Ta49Ti, Nbl8Ta39Ti, Nbl7Ta44Ti, and Nbl5Ta5lTi were encapsulated in conductive mounting compound (PSI-212-1). EMPA was done in The College of Oceanic and Atmospheric Sciences at Oregon State University. Two scans were made of each of the samples examined. The line measurement consisted of ten point analyses evenly spaced along a 10 tm line. The random measurement chose 10 points randomly from the filament crosssection. 17 Annealing Conditions: The second set of as-received samples was prepared basically in two groups. One group was prepared in our Lab while the other set was prepared in the Chemistry Department at Oregon State University. All samples were cleaned and wrapped in the zirconium foil and then placed into a quartz tube. One end of the quartz tube was sealed and the other end of the tube was connected to a mechanical vacuum pump. Samples prepared in our lab were placed at the sealed end and continuously evacuated for about 36 hours before placing in the tube furnace for the heat treatment. The quartz tube with samples in it was then put into the oven at the specified temperature for 300 hours. After turning off the oven, the pump was kept pumping until the samples cooled down (generally this took about another 24 hours), and then the samples were taken out. Investigated binary and ternary samples and heat treatment schedules are listed in Table 7 below: Table 7. The sources of samples and their heat treatment conditions BINARIES Samples Composition (wt. %) Annealing Conditions NbTi 46.5Ti (bulk) 400°C/300h 450°C/300h 500°C/300h 550°C/300h Ta5OTi 46.5 Ti (wire) 400°C/300h 450°C/300h 500°C/300h 550 °C/600h 55Ti (bulk) (bulk) 400°C/300h 450°C/300h 500°C/300h 550 t/600h 400°C/300h 450°C/300h 500°C/300h 550 CI300h 600 t/600h 600 °C/600h NB-TI-TA TERNARJES Composition (wt. %) Annealing Conditions l2Ta46Ti l5Ta5lTi (multi-) (mono-) l7Ta44Ti (mono-) (bulk) 24Ta49Ti (mono-) 28Ta4lTi (mono.) 400°C/l000h 450 °C/300h 500 "C/300h 550 °C/600h 400°C/l000h 450 °C/300h 500 'C/300/j 550 °C/600h 400°C/l000h 450 C/3OOh 500 "C/300h 550 °C/600h 400°C/l000h 450 °C/300h 500 °C/300h 550 °C/600h 400°C/l000h 450 °C/300h 500 'C/300h 550 C/600h 400°C/l000h 450 °C/300h 500 "C/300h 550 °C/600h 600 °C/600h 600 °C/600h 600 t/600h 600 °C/600h 600 °C/600h 600 °C/600h The samples in italic are evacuated by argon. multi-: means the samples were in multi-filimentary form mono-: means the samples were in mono-filimentary-form l8Ta39Ti 18 After heat treatment, samples with active pumping were slightly surface-oxidized, depending on the annealing temperature. In order to remove the oxidized layer, samples were surface-polished and cleaned again. Those samples prepared in Chemistry Department were evacuated as we did in our lab. The samples were then being back filled with argon gas in order to get rid of the oxygen contamination. After being back-filled with argon gas, the quartz tube was sealed at the open end too. After heat treatment, all bulk samples were filed into powder using a fine file. The wire samples were cut into tiny pieces. All samples were mounted within sample holders for the XRD measurement. Two types of sample holder were used. One was 25-mm in diameter with Vaseline as an adhesive material, the other one was 6 mm in diameter with double-sided tape as the adhesive material. Experimental results showed that there was no significant difference between XRD results from these two types of sample holders. All ternary samples, binary Ta5OTi and Nb55Ti at 600°C and Nb46.5 Ti at 550°C were back-evacuated under argon condition except at 400°C. X-Ray-Diffraction Analysis: X-Ray Peak Fitting Routine Diffraction Patterns were recorded using a Siemens D5000 diffractometer. In all cases the intensity measurements were made at room temperature with a Cu Ka (al 1 .54O6A, a2=1.5443X) x-ray source. The data was collected over the 20 ranging from 35 degrees to 100 degrees because the highest intensity peaks of both a-Ti HCP and p-Nb/Ta BCC phases lie in this range. The x-ray was scanned at a step size of 0.01 and 0.02 degree using a step-counting time between 1 second to 3 seconds. The peaks in diffraction intensity at 0 K are governed by Bragg's Law: n X= 2 d sin0, where n is an integer, X is 19 the x-ray wavelength, d is the spacing between atomic planes, and 20 is the scattering angle in the plane of the source and detector. At the most basic level, XRD may be used to determine the lattice parameter (X, 0 are known), crystal structure (we weren't concerned with it here), and phase composition (as described in Appendix i). The observed x-ray diffraction patterns were modeled by a Gaussian function or a Lorentzian function, and fit using a least squares fitting program in order to determine the peak shapes and correct for peak overlap. The refinement was performed assuming n diffraction peaks (we set up the maximum number of fitting peaks to five, but it's easy to change the program), and the fitting parameters of each peak were a) offset of the background; b) peak position; c) full-width-half-maximum (FWHM); and d) intensity. In our experience, the Lorentzian function fits the data better in most cases. This may be attributed to the interesting characteristics of Lorentzian distributions. The Lorentzian function does not diminish to zero as rapidly as in Gaussian's distribution, so it can pick up data along the "tail" and therefore gives the better fitting result. This program is almost user independent. X-ray data analysis routine Using the peak-separated and fit XRD data, an intensity ratio of the a to f3 phase was obtained, as well as the Lorentzian factors, structure factors and multiplicity factors (see Appendix I for details). Once C/C is found, the value of C can be obtained from following relationship: laRfi RaCa I RCfl C, Equation 2 IpRa The additional relationship C+C= 1 is used together with above equation to get the composition of both phases. After the compositions were obtained, the lever rule was applied to calculate the mass fraction of certain phases. 20 c -cA Ma = /3 Equation 3 Where: M is mass fraction of phase calculated from concentration of element i, C' is 13 the concentration of element i in 13 phase, C is the concentration of element i in a phase and CA is the overall concentration of element i in the alloy. Critical temperature measurement: The critical temperatures were measured using a Tc probe built by Dr. Warnes and previous graduates in the Cryogenic Lab. In this probe, there are three coils: excitation coil, pic.k-up coil, and a set of witness coils. The schematic of critical temperature measurement is shown in Figure 4. The excitation coil at the bottom of the probe is used to produce a magnetic field around the sample. Pick-up coil on the top of the probe is aligned with excitation coil and used to pick up the signal. The sample will be sandwiched in between. The witness coils were composed of Nb coil and Pb coil connecting in series and used as calibration coil due to the fact that Tc of pure Nb and Pb are known to be 9.3 K and 6.9 K respectively: The Cemox thermometer is embedded into the probe in order to control the temperature around the sample. The heater is wound all way around the aluminum plate sample holder, and thermometer in embedded into the aluminum plate. The details are described in report [21 The measurement uses the Messiner effect mechanism which says that after superconducting material is cooled down below it's Tc, the magnetic lines can't pass though the superconductor any more. Or in other words, the superconducting materials will shield the magnetic field out when it is in the superconducting state. 21 Pick-i.p Coil Nb Ninss CniI Dx ieter Pb Witness Coil Loll Temperature Block Figure 4. The schematic of critical temperature measurement. The probe is composed of an excitation coil at the bottom of the probe and used to produce a magnetic field. The pick-up coil on the top of the probe is aligned with excitation coil and used to pick up the signal. The two other coils: Nb and Pb coils connected in series and are used to calibrate the data later on. The Cernox thermometer is embedded into the probe in order to control the temperature around the sample. 22 RESULTS AND DISCUSSION The Nb-Ti, Ta-Ti binary and Nb-Ti-Ta ternary equilibrium phase diagrams all exhibit a two-phase equilibrium between a-HCP, and 13-BCC phases. The temperature of the cYA=f3 transformation of titanium gradually decreases with increase in the concentration of niobium and tantalum. At the titanium apex of the ternary triangle diagram there is a small region of a solid solution based on the titanium and bordering on the two-phase region (a+f3). EMPA Results on Sample Homogeneity: From the EMPA data (see Table eight), we can see that titanium has the biggest variation. The most concern is on the Ta due to its high melting temperature and might least be melted. In contrast, the Ti is the most likely to disappear during the melting. All three elements show a variation of less than 1 wt%. This indicates a reasonable homogenous starting sample. EMPA data for two of the samples (Nb46Til2Ta and Nb4lTi28Ta) are lacking. Table 8. Chemical analysis of ternary samples using electron microprobe analysis. All compositions are given in weight percent. NbSlTil5Taline Nb5lTil5Ta random Nb44Til7Ta line Nb44Til7Ta random Nb39Til8Ta line Nb39Til8Ta random Nb49Ti24Ta line Nb49Ti24Tarandom Nb avg. 33.85 34.00 39.62 39.48 42.97 43.09 27.39 27.31 Nb Stddev Ta avg. Ta Stddev ±0.27 14.97 15.00 17.94 17.40 19.61 18.49 22.75 ±0.35 0.14 0.38 0.42 0.20 0.19 0.25 ±0.35 23.12 ±0.75 ± ± ± ± ± ± ± ± ± ± ± ± 0.32 0.33 0.75 0.70 0.74 0.67 Ti avg. 51.47 50.81 42.52 42.52 37.39 38.41 49.64 48.94 Ti Stddev ±0.55 ± ± ± ± ± ± 0.71 0.62 1.06 0.80 0.82 0.94 ±0.76 23 Binary Alloy Systems X-Ray Diffraction Results The x-ray diffraction data of Ta-Ti and Nb-Ti at different temperatures are shown in Figures 5 and 6 respectively. In Ta-Ti, at low heat treatment temperatures there is not a distinct separate 40°a-peak. The a-phase peak starts to become obvious at 500°C, and becomes even more distinguishable from the 3-phase peak at 550°C. This indicates the diffusion rate becomes faster at 500 °C, and faster yet at 550°C. In the Nb-Ti binary system, the XRD pattern is less obvious than that in Ta-Ti system, even at 500°C(Figure 6). This suggests that Nb-Ti has a more sluggish diffusion rate than that in Ta-Ti. The diffusivities will be discussed later. NbTi bulk samples didn't show obvious traces of the two phases. However, the 40-degree a-phase peak appears in heat-treated wire samples at 500°C and 550 °C, as shown in Figure 6. At 550°C, the 63 degree a-Ti peak appears too. Using longer scanning time and smaller step size, the 40-degree peak can be seen, but it is quite small at 550°C. This indicates wire samples have much faster kinetic than the bulk samples. However, the composition point we tested is so close to the 3-phase boundary at 550°C, and the volume fraction of a-Ti is very small, and therefore results a very small intensity peak. 24 700 600C 600 550C 400 500C 300 200 450C - 100 0 35 40 45 50 400C ---r-I-1t- -----.--1r'rri.-*l1 55 60 70 65 75 Diffraction Angles (2 theta) Figure 5-a. Tantalum-titanium x ray diffraction pattern for different temperature heat treatments. The 40 degree alpha peak becomes obvious starting from 500°C, as well as 55 and 70 degree peaks. The intensity of 600 °C shrinks, as well as the alpha phase peak at 40 degrees. The small angle and long time run for 600 °C shows that alpha phase peak at 40 degree is still visible. All sample data here are taken at 0.O2dgIs. 250 - 200 150 100 01 . 50 36 37 38 39 40 41 42 Diffraction Angles (2 theta) Figure 5-b. Tantalum-titanium XRD pattern for a 600°C heat treatment. This was obtained by step-size of 0.01 dg/2s. 25 800 700 600 C ? 500 0 0 400 300 200 100 0 35 40 45 50 '- 55 60 -65 70 -' 75 Diffraction Angles (2 thetcO Figure 6. Typical Niobium-titanium samples XRD pattern under different heat treatment temperatures. Even though distinct separate a- and J3- phase peaks do not always appear in the XRD data, the asymmetric peak near 40 ° can be analyzed as two separate overlapping diffraction peaks. To find the individual peak intensities, the XRD data were analyzed by a custom peak fitting routine. The results are shown in Table 9. The intensity ratio of f phase to a phase of TT start to rise from 500 °C, but shrank at 600°C. This indicates that diffusion rate rise up at 500°C. At 600 °C, although the kinetics is faster, the V% of a-Ti ppt is smaller, and therefore the intensity peak ratio is smaller too. Unfortunately, we were not able to get the experimental data at temperatures higher than 650 °C for Ta-Ti due to the sample composition limitation. From TaTi binary 13-phase diagrams, it is seen that at a composition of Ta50 wt%Ti, the 650 °C is in a single 13- phase region. We don't have experimental data to present at temperatures below 450°C. Actually, it is almost impossible to get this system to equilibrium at such temperatures within our lifetime. However, thermodynamic calculations allow us to extend our work to where the experiment couldn't reach, as discussed in the next section. Table 9-a. Ta-Ti X-Ray Diffraction Data Beta-Phase lorentz-polarization factor 20 hkl 38.88 55.97 70.2 200 6.8016 2.6107 12 6 211 1.4301 24 38.90 55.99 70.20 110 6.7930 200 2.6081 1.4242 12 6 38.74 55.94 70.32 200 110 211 110 211 multiplicity factor 24 6.8625 2.6146 1.4182 12 6 24 structure factor Intensities 58.1933 50.9756 46.0275 72.39 21.41 28.15 58.1843 50.9679 45.9897 220.1 25.37 58.2566 50.9872 45.9513 234.6 37.07 65.87 structure factor 14.0120 Intensities 11.9937 9.9965 6.180 22.16 44.24 Phase hid lorentz-polarization factor 6.3623 multiplicity factor 39.94 53.10 70.69 101 102 103 3.0171 1.4006 40.29 53.13 70.68 101 102 103 6.7930 2.6081 1.4242 12 12 12 13.9525 11.9896 9.9974 38.17 6.56 28.49 40.16 53.18 70.62 101 6.8625 2.6146 1.4182 12 12 12 13.9797 11.9842 10.003 46.32 102 103 12 12 12 14.44 10.16 18.52 Table 9-b. Nb-Ti X-Ray Diffraction Data Beta-Phase lorentz-polarization factor 20 hid 38.88 55.97 70.2 200 6.8016 2.6107 211 1.4301 38.90 55.99 70.20 110 200 6.7930 2.6081 1.4242 12 6 38.74 55.94 70.32 200 6.8625 2.6146 1.4182 12 6 110 211 110 211 multiplicity factor 12 6 24 24 24 structure factor Intensities 58.1933 50.9756 46.0275 72.39 21.41 28.15 58.1843 50.9679 45.9897 220.1 25.37 58.2566 50.9872 45.9513 234.6 37.07 65.87 structure factor 14.0120 11.9937 9.9965 Intensities 14.44 6.180 22.16 44.24 Alpha-Phase lorentz-polarization factor 6.3623 20 39.94 53.10 70.69 hid 102 103 3.0171 1.4006 12 12 12 40.29 53.13 70.68 101 6.7930 2.6081 1.4242 12 12 12 13.9525 11.9896 9.9974 38.17 6.56 28.49 40.16 53.18 70.62 101 6.8625 2.6146 1.4182 12 12 12 13.9797 11.9842 10.003 46.32 101 102 103 102 103 multiplicity factor 10.16 18.52 28 As we know, two factors influence the position of the phase boundary. One is the alloy composition, as discussed in the Introduction. Iii Nb/Ta-Ti, the n-phase boundary drops to the lower temperature when the f3-phase concentration becomes higher in Nb or Ta. In other words, for a fixed alloy composition, increasing the temperature is equivalent to decreasing the Nb/Ta content of i phase boundary. The other factor that affects the B- phase boundary is the interstitial content [71 This might be an important factor, but is not included in this work. Phase Diagram Calculations by the Regular Solution Model The calculation of the binary phase diagram based on the regular solution model is expressed using: = (1 x)F'+ XF1a+ RT{xlnx+(l x)ln(1 x)]+ (cal/g-atom) Equation 4 Where Fu is the free energy of the a phase, Fa and Fa are the free energies of the a forms of pure i and j, and Ea is the regular solution excess free energy, and can be expressed as E = Bx(1 x), where B is interaction parameter for bcc phase in the i-j system. The detail is described in Appendix II. Generally, the interaction parameters are determined by experimental data. In this work, interaction parameters were adopted from Kaufman's [11] work for titanium alloys. These parameters from Kaufman together with parameters obtained from Chernov' s work261 are listed in Table 10. The calculated phase boundary, as well as some other reference data, is listed in Table li-a for TaTi and Table 11-b for NbTi binaries respectively. 29 Table 10. Regular solution parameters for Ti-based stable equilibria Interaction Parameters Interaction Parameters BCC Ti-Ta Ti-Nb Sources B=3324 B=2790 B=3200 B=3125 [26] [11] HCP A=3370 A=2790 A3700 [261 A=3125 [11] Stability Parameters LFT?(T) = -1050+0.91T FNb/a(T) = 1500+0.8T [11] [111 Table 11-a. The tantalum-titanium binary phase boundary Temperature Ta wt. % of ct-phase boundary Ta wt. % of 3-phase boundary iocr c 0j6b 9975b 079b 259b 9786b 200CC 300 C 400 °C 450 °C 500 °C 550 °C 6.94[18], 5b 600°C 11.87[171, 11.05 650 °C 700 °C 800 °C 10[18] 882.5CC [26] [18] 91.69a, 91.7[18] 8.36 9.8 [18] 939b 1 1[18], 12.15 [17], [17] 128b 10.75 9.8 [18] 797[17] 5.1E18], 1079b 038b [18] 9512b 4a 83.4 [18], M9b 93.8 [26], [18] 67.12a, 56.94a, 67 65.56 [16], 62 [18] 60.69 [271, 5518b 48 [18], 61.83 [16] 35.06 [26], 36.5 [18] 3613b 50 [17], 58.3 [16] [18] 1723b [17] 28.9 43.63 8.83 [26], 13.5 [16], 038b a XRD data, predicted data by thermo-cal. All data from this work has been underlined. 30 Table il-b. The niobium-titanium binary phase boundary Temperature Nb wt. % of a-phase boundary Nb wt. % of 3-phase boundary 100 C 200 C 989b 300CC 375 °C 380 °C 60[19] 400°C 420 °C 450 °C 500 °C 550 °C 600 °C 650 °C 680 °C 700 °C 725 °C 765 °C 800 °C 810 °C 37[20] 6312L35], 5595(18] 411[18]4,b 5495 [18]93 95b 58[42], 62[23], 64(41] [18] 85.75a, 46.47(18] 72.19a, 40 [18], 8637b [18] 6o6' 33.0 [18] 4.25[18] 4.1 [18] 4173b 28.05 [18j 22.8 [18] 3.68[18], 32.67(8] 3.1 [18] 57b I .42[18], 30b [18] 15.5 25.51(8] 17.74[8] 6.2 [18] 9.27[8] 882.5CC 885 °C a XRD data, 0(81 predicted data by thermo-cal. All data from this work has been underlined. 31 Ref.18 ''- Ref. 45 800 yRn 700 600 a 400 300 200 100 0 20 40 60 80 100 Weight percent of tantalum (wt.%) Figure 7. The binary Ta-Ti alloy system at low temperatures. The solid thick lines indicate the standard binary phase diagram [18] The solid thin lines show the calculated phase boundaries from the regular solution model calculations. The circles show the XRD results from this work. 900 Ref. 18 800 Ref 45 300 200 100 0 20 40 60 80 100 Weight percent of niobium (wt. %) Figure 8. The binary Nb-Ti alloy system at low temperatures. The black lines indicate the standard binary phase diagram1181. The grey lines show the calculated phase boundaries from the regular solution model calculations. The circles show the XRD results from this work. 32 In TaTi binary system, our XRD data agrees with our predicted B-phase boundaries, as well as to the published one at a temperature <500°C and> 700°C very well, see Figure 7. But end up with a lower tantalum content for beta phase than ASM data at 550°C and 600 °C. The calculation, as well as all experimental data from the literature of beta-phase boundaries is shown in Table 11. As we mentioned before, thermo-calculation allows us to extend our work to where the experiment couldn't reach. The f3 phase boundaries of Ta-Ti and Nb-Ti binary systems are thermodynamically predicted at all temperatures and compositions. There are only two sets of data for Ta-Ti at temperatures lower than 450°C. Both works approach this issue by using the regular solution model. One is from Chernov's work [26], and the other one is from this work. The difference of our results and Chernov's is very small at low temperature. However, our results at 450 °C and 500°C are closer to both XRD ones and the published ones than Chernov's. The stability parameters and interaction parameters can be determined by the presence of positive values of the excess thermodynamic potential , which correspond to the last term in equation (4), whose numerical characteristic is the value of the interaction parameter in the phase considered, details are explained in Appendix II. The positive values of the parameters are indicative of the tendency of these systems to demixing. Chernov' [26] results, as shown in Table 10, are similar to the data from Kaufman [h11 However, Chernov uses larger interaction parameters and a difference between B-phase and a-phase interaction parameters. This is why their results have a higher tantalum content 13-phase boundary at 400 °C and 500°C, and a smaller tantalum content 13-phase boundary at 800°C. Larger positive interaction parameters always show wider two-phase fields. But their results agree with the published data at 600 °C and 700 °C pretty well, and the discrepancy is less than 1%. 33 Contamination Effect As we mentioned in the Introduction, Summer's and Maykuth's 3-phase boundaries have much higher Ta content than all other works. The reason is the most possible due to the contamination. No experiments have been carried out to determine the extent of the solubility of Ta/Nb in a-Ti. Our n-phase boundary of Nb-Ti binary that is predicted by the regular solution model and XRD results has a higher Ta solubility at higher temperature than ASM [1 8J No experiments have been carried out on the effect of contamination in determining the 3-phase boundary. However, a lot of effort has been put on clean sample preparation in order to get rid of the contamination. Following are the facts that imply our 3-phase boundary is not due to the contamination: 1. The Nb-Ti and Ta-Ti binary samples are under same heat treatment conditions. Ta-Ti binary phase diagram shows a good agreement with ASM standard, as well as to all other references. So, our Ta-Ti is free from contamination, same as Nb-Ti samples. 2. All samples without Ar back-filled shows the oxygen layer, even at low temperature (400°C). However, not a single sample under Ar back-filling shows the oxygen layer, even at high temperatures, such as 600°C Kinetics of B and a Transformations The kinetics must be considered when evaluating the experimental phase diagram data. In an alloy like TaTi, the diffusion coefficient of interest is the interdiffusion coefficient. The diffusion coefficient of the TaTi system was measured by Ansel 461 using TaTi diffusion couples and Ta/TaTi pellet. The data was collected over a temperature range of 1000° C to 1900°C. The interdiffusion coefficients were calculated from concentration 34 profiles determined by EMPA. There are several characteristics about TaTi diffusion [471, and they are summarized as follows: a. In the same way as other Ti alloys, the diffusion coefficient increases exponentially with increasing temperatures and decreasing B-stabilizer (tantalum) content. b. The Arrhenius plot of mD vs lIT does not give a straight line, but curved. At low composition, the plot has a disperse trend with decreasing the temperature, and D and Q increase with Ta content. By using D=D0 exp(-QIRT) to fit the data, the activation energy and frequency factors have a maxima around 35 at % to 40 at % of Ta [461 The Arrhenius plot converges after 35 at % with decreasing the temperature, and D0 and Q decrease with tantalum content. The discontinuity (around 35 at %) is considered as a change of the diffusion mechanism, called the crossover point. Before this point (35% composition), one diffusion mechanism dominates the diffusion system, but it doesn't mean there is only one diffusion mechanism operating. Over the whole range, there may be two or more diffusion mechanisms existing. The curvature of the Arrhenius plot suggests an increase in the activation energy and frequency factors with temperature. Therefore neither D0 nor Q are constant. According to these characteristics, it will be more reasonable to consider two or more diffusion mechanisms in this system, instead of fitting all data into one equation over such wide composition and temperature ranges. For refractory alloys, a suggested [48] two diffusion mechanism model is proposed as follows: D= D1-i-D2 where D1 =D01 Equation 5 exp(-Q1IRT), D2 =D02 exp(-Q2JRT), D is interdiffusion coefficient, in the unit of cm2/s, D01 and Qi versus D02 and Q2 represent the different diffusion mechanisms, and this will be discussed further later. Here, the D0 is in the unit of cm2/s and Q is in the unit of J. We consider this transition point as the separation point for different diffusion mechanisms, and obtain D01 Qi, D02, Q2 as follows: 35 1.OE-06 a-.--. o 4.-- 10 1.OE-07 ---à--- 20 -- 30 4*--- 40 1.OE-08 50 -0----. 70 -0---.- 80 1.0E-09 l2 I---- 90 = 1.OE-10 ! 1.OE-11 1.0E-12 1.OE-13 4.5 5 6 5.5 6.5 7 7.5 8 1000ff (1/K) Figure 9. Semilog plot of the diffusivity as a function of the inverse of the temperature for Ta-Ti binary alloy. The lines show diffusivity at different compositions (weight percentage). 1000 900 800 I- 700 E .1 600 500 400 0 20 40 60 80 100 wt % Ta Figure 10. Comparison of interdiffusion coefficients of Nb-Ti and Ta-Ti binary systems. The Ta-Ti diffusivity (in the unit of cm2/s) is higher than that in Nb-Ti binary at same temperature and compositions. At 550 °C, our Ta-Ti samples (50 wt.% Ta) is around 5 order of magnitude higher than that of Nb-Ti (53 wt. % Nb) binary. D01= 9E4*exp(0.0575 *x) [cm"2/sj, Q=3623 8 *exp(00 125 *x) (0<x<30) D02 = 4E4*exp1\(0.0612*x), Q2 =78063*exp(0.0092*x) (35<x<90) The modified Arrhenius plot of mD vs. 1000/T, as shown in Figure 9, is a group of straight lines. This indicates a better fit by using two-diffusion-mechanism model. The diffusion rate of Ta-Ti and Nb-Ti are compared in Figure 10. Nb-Ti data is taken from Moffat' s thesis [71 The Ta-Ti system has three or four orders of magnitude higher diffusion rate than that of Nb-Ti. For instance, the diffusivity of Nb47Ti at 450°C is about 1E-21m2/s, and about 1E-18 cm2/s in Ta47Ti. The diffusion rate of Nb47Ti and Ta47Ti at 550°C is 1E-20 cm2/s and 1E-16 cm2/s. This means that if Ta-Ti can reach the equilibrium state at 450°C in 24 hours, it probably will take 1000 days for the Nb-Ti system to reach the equilibrium state. This is why we have clearly defined Ta-Ti a-phase peaks, but not in NbTi at the same annealing conditions. Conclusions: For Ta-Ti binary alloy, our experiment data, theoretically predicted 13- phase boundaries are very close to ASM published data, as well as to the most of the reference data. However, both our experimental data and theoretical predicted data in TaTi binary alloy show an obvious higher J3-phase boundary than ASM published results. However, our experimental data and our predicted results are self-consistent. Ternary Alloy Systems The Nb-Ti-Ta ternary alloy phase diagrams are determined using regular solution model calculation and XRD, and the final phase diagram is extrapolated according to experimental results. Ternary samples and Adopted Model Figure 10 shows a ternary phase diagram and the six as received ternary samples investigated. Comparing this diagram with Figure two in the INTRODUCTION, it is not 37 hard to see that out of six ternary samples, only two of them ( Nb28Ta4lTi and Nb24Ta49Ti) can really be driven to the high H2 after heat treatment. The As-received samples are distributed all around the H2 peak (around 400 °C to 600°C). Only if 13- phase is in convex shape, all samples will be in the a+13 two phase region, and will be useful to do phase analysis under all precipitate temperatures. Ternary Alloy Phase Diagrams Thermo-Calculation phase Diagrams The ternary phase diagram predicted by first principle calculation based on the regular solution model that is described in detail in Appendix II is displayed in Figure 11. At all temperatures, the 13 phase boundaries are in concave shape, as expected before However, a smaller a+f3 intermediate phase region is resulted. One thing that needs to be mentioned is that in the ternary alloy system, more assumptions were made in the calculation due to its more complicated interactions, and it is therefore much more uncertain. X-Ray Diffraction Results Evaluation of the ternary phase diagram according to the XRD is shown in Figure 12. From Figure 12, we can see that the phase boundaries at different temperatures have different shapes. The 550°C one is more convex and 400 °C one is more concave in shape. The 400°C one is nearly lying on top of the 450°C one. When diffusion kinetics are considered, there is about four orders of magnitude difference of diffusivity between these two temperatures. This strongly suggests an insufficient heat treatment time used for 400°C. A rough estimation of the heat treatment time used for 400°C to reach equilibrium is about 10,000 times longer than that used for 550°C. Therefore, the 550°C 38 XRD data is more reliable to represent the phase boundary. Based on the 550°C data, an extrapolated ternary phase diagram is therefore built, as shown in Figure 13. Nb 470 520 540 /: 0 samples 555 4I 400C 580 5OOC 605 \,/ \ 600c Ta Figure 11. Type B ternary phase diagram and investigated samples which showing the starting alloy compositions studied in this work (empty circles) and the calculated 13phase boundary at 400, 500, and 600 °C using regular solution model. Table 12-a. The niobium-titanium-tantalum ternary 3-phase boundary-XRD NbTiTa wt. % of 3-phase composition Starting alloy 400°C 1246 3329 1551 1774 1839 2449 2841 450°C 2422 2921 2038 1939 500°C 550°C 1535 2139 1936 2129 600°C 39 Table 12-b. The niobium-titanium-tantalium ternary 3-phase boundary-Calculation NbTaTi wit. % of p-phase composition 400°C 500°C 600°C 88.09Ta8.27Ti 87.26Ta8.75Ti 55.7Ta29.95Ti 51 .32Ta32.38Ti 47.33Ta34.43Ti 43.43Ta36.3Ti 30.65Ta41 .57Ti 17.44Ta45.9Tj 18.91 Ta54.22Ti 30.85Ta49.64Ti 38.69Ta46.21 Ti 47.93Ta41 .59Ti 55.77Ta37.O8Ti 1 5.98Ta64. l3Ti 24.07Ta60.9Ti 29.49Ta58.56Ti 40.74Ta53. l6Ti 53.29Ta46.OlTi 60.66Ta33.95Ti 65.43Ta30.64Ti 82.26Ta17.27Ti 0 470 A 5500-oOOh-XRD 400C-l000h-XRD 520 / 540 z\ 555 580 605 800 Ti 4500-300h-XRD /\ /\/ '///T/\/\ _"/i \ U 5000-300h-XIRD o000-oOOh-XRD 4"""4000 boundary "4 5500 boundary - 650 720 / - starting alloy / \ /\ /\ /\ /\ /\ ' Ta Figure 12. Experimental data from precipitating heat treatment at different temperatures in Nb-Ti-Ta ternary alloy system. The hollow circles are as-received samples. All others are XRD data from different treatment temperature and times. Notice there are some overlaps for 550°C data and 450°C data. 40 stcifingdloy 470 L 45OCExtrqxIc*ion -.--- 500C E xtrqxldion *H 550C E xtrqxIation + ÔOOC E xtrcoIation 650C Ext rcpxt ion 580/ Ta Ti ..1 .1I ' QO QO JI U U ,JI Figure 13. The extrapolated ternary equilibrium phase diagram for the Nb-Ti-Ta system. The dotted lines mark the extrapolated position of the f3-phase boundary at 450, 500, 600, and 650°C. The solid line at 550°C is the experimentally determined 13-phase boundary from the quantitative XRD analysis. The solid line near the Ti apex is the approximate aphase boundary. For this work, the assumption was made that the a-phase boundary was independent of temperature. Diffusion Behavior of Ternary Alloys The diffusion rates of Nb-Ti-Ta ternary at different temperatures are estimated based on the binary data, and are shown in Figure 14-16. At 400°C, the 13 phase boundary is located below diffusion coefficients of 1E-20 cm2/s, and has diffusivity of about 1E-21 cm2/s. At 500°C, all samples are within the range of 1E-20 cm2/s to 1E-18 cm2/s. From these diffusion plots, a heat treatment time and precipitate size can be estimated. Compared with similar composition of binary samples, the diffusion rate of ternary samples (Nb5iTil5Ta and Nb49Ti24Ta) at 400°C are very close to that in TaTi. The aprecipitate size after the heat treatment is estimated to be about 100 nm in diameter in ternary alloy system. The a-precipitate size is about 3 to 5 times larger than that in the Ta5OTi binary system based on the estimation from diffusion length X='JDt. 41 Nb starfing alloy C) - 470 E-20 (cm"2/s) - - - E-18 (cmA2/s) 520 E-lo (cm"2/s) - 540 E- 14 (cmA2/s) 555 580 605 720 '-S Ti 800 C Ui - = '' th à C Ui Ta Ui Ui Ui -4 Figure 14. Ternary diffusivity-Lines of constant diffusivity plotted on the Nb-Ti-Ta ternary phase diagram at a temperature 400°C. The inter-diffusivity coefficient extends over a range from 1014-1020cm2s. Figure 15. Ternary diffusivity-Lines of constant diffusivity plotted on the Nb-Ti-Ta ternary phase diagram at a temperature 500°C. The inter-diffusivity coefficient extends 42 over a range from 10'4-1020cm2s. Nb starting alloy 470 - E-20 (cm"2/s) 520 - - - E-18 (cm"2/s) E-lo (cmA2/s) 540 E-14 (cm"2/s) 555 E12(cmA2/s) ......... 580 605 650 720 N .., ...' N Ti Figure 16.Ternary diffusivity- Lines of constant diffusivity plotted on the Nb-Ti-Ta ternary phase diagram at a temperature 600°C. The inter-diffusivity coefficient extends over a range from 1012 1020cm21s. Critical Temperature For Binary and Ternary Alloy Systems Critical temperature measurements were carried out by an inductive method. Temperatures were measured by Cernox RTD thermometer with 0.005 precision. Inductive measurements were implemented at a frequency of 500 Hz. Generally speaking, the resistively measured Tc values are higher than inductively measured ones, although both follow a similar trend. The resistive method probes the best one dimensional superconducting path, whereas the inductive method provides more of a volume average of Tc transitions. Resistive transitions are about 0.1 K wide according to Suenaga, inductive transitions are around 0.35K, or even more in our case. Other effects that may influence Tc are the annealing time and annealing temperature. The higher the annealing temperature and the longer the annealing time, the higher the 43 transition width of Tc, as shown in Appendix III. The increment of transition width with aging time is attributed to niobium enrichment of the matrix that accompanies the o-Ti precipitation and incomplete diffusion in the 3-phase. The measured critical temperatures of fifty-eight samples are listed in the table in Appendix III. The critical temperatures vary from 6.65 K for As-Received Ta5OTi to 10.77K for Nb55Ti heat treated at 500C for 112 hours, and the transition width varies from 0.04 K to 1.94 K. Some of our transitions are really wide compared with Suenaga's data. Especially for Nb46Til2Ta ternary samples, the average width of this composition of eight samples is 1.22 K. The reason for that is not clear yet. Our other four ternary samples have a very good homogeneity according to the EMPA results though. Our Tc data is plotted on top of Suenaga' s plot, converted to weight percentage of compositions, as shown in Figure 17. The transition temperatures of a-Ti or martensite a" phase are low, and observed Tc for any given alloy depends not on the average composition of alloy but on Tc of highest Tc phase present, the BCC-f3 phase. It is noticed that the Tc data for 400 °C-l000hrs is less valuable. Although they are under the longer annealing time, the kinetics of these ternary samples depends on temperature more than time, as we discussed before. Therefore, the Tc data at 400 °C is less reliable. 44 Nb-Ti-Ta Tc Pfot Nb 550C X 40CC-i 000h 450C-300h A 55CC-oUCh T I -600C-000h a TI -,AJ x 1551-400C-l000h Ta Ti 66 7.29 8.14 8,59 7.98 Figure 17. Critical temperature as a function of alloy compositions. The lines represent the data of Suenaga and Ralls301, while the data points indicate the measurements of this work. The compositions given are composition of 3-phase for heat treated alloys. Conclusions: From the detailed study of metallurgy of Nb-Ti-Ta ternary and it's binary systems, following conclusions are drawn: 1. A working ternary equilibrium phase diagram for the Nb-Ti-Ta system has been developed that is based on experimental measurements and quantitative thermodynamic calculations. The ternary phase diagram can be used as a metallurgical tool for ternary alloy development and design of ternary alloy processing. 2. Evaluations of the thermodynamics and XRD measurements of the Nb-Ti and Ta-Ti binary systems have led to improved versions of the equilibrium binary phase diagrams. In particular, the Nb-Ti phase diagram developed here shows the 45 3-phase boundary at higher temperatures and lower Ti compositions than the presently accepted phase diagram. Measurements of the superconducting critical temperature, T, show good agreement with previous measurements of Tc in the ternary alloys. Changes to the Tc as a function of precipitation heat treatments cause the Tc to follow the composition changes in the n-phase as Ti precipitation occurs. In the alloys and heat treatments studied here, the Tc remained above 8K, which should result in minimal impact on applications for the ternary alloys in magnet systems. 4. Coupled with previous information on the expected Hc2 behavior of the ternary alloys, the phase diagram and T data indicate that there is still reason to expect the Nb-Ti-Ta ternary system is capable of reasonable properties for high field magnet applications at temperatures below 4.2K. BIBLIOGRAPHY 1 W. H. Warnes and N. Li, Adv. Cryogenic Engr., 46:923-930 (2000). 2 W. H. Warnes and N. Li, -A Continuation Final Report, final report submitted to Fermi National Accelerator Laboratory, (September, 2000). 3 Joint Committee on Powder Diffraction Standards (JCPDS)-International Center for Diffraction Data (1998). 4 E. K. Moichanova, Phase Diagrams of Titanium Alloys. Jerusalem, Israel Program for Scientific Translations, D. (Davey, New York. 1965). 5 P. J. Lee, Encyclopedia of Electrical and Electronics Engineering, 21:75-87, New York: John Wiley & Son, Inc., (1999) 6 B. D. Cullity, Elements of X-Ray Diffraction, Addison-Wesley Publishing Company, Inc. Reading, Massachusetts (1978). 7 D. L. Moffat, Ph.D Thesis University of Wisconsin, Madison, (1985). 8 M. Hansen, E.L. Kamen, H. D. Kessler, and D. J. McPherson, Trans. AIME, J. Metals, October: 88 1-888 (1951). 9 Brown, A. R. G., Clark, D. Eastabrook, J. and Jepson, K. S. Nature, 210:914-915 (1964) 10 J. L. Murray, Phase Diagrams of Binary Titanium Alloys, ASM, Metals Park, OH (1987) 11 Kaufman, L. and Bernstein, H., Computer Calculations of Phase Diagrams, Academic Press, New York (1970). 12 Imgram, A. G., Williams, D. N., Wood, R.A., Ogden, H. R., and Jaffee R. I., WADC Tech Rept (Wright Air Development Center. Technical Report):59-595, Part 11(1961). 13 Ronami, G. N., Kuznetsova, S. M., Fedotov, S. G. and Konstantinov, K. M. Moscow Univ Phys Bull, 25(2): 55-57 (1970) 14 R. Krishnan, S. P. Garg, N. Krishnamurthy & E. Paul, Journal of Alloy Phase Digrams, 3 (1):28-30 (1987). 15 D. S. Summer. Journal of Institute of Metals. 81: 73 (1952-1953). 16 D. S. Summer, Journal of Institute of Metals. 8 1:426 (1952-1953). 47 17 D. J. Maykuth, H. R. Ogden, R. I. Jaffee, J. of Metals. February : 231 (1953). 18 T. Massaiski, ed., Binary Alloy Phase Diagrams, ASM International, Metals Park, OH (1990). 19 Liu H. and E. Gregory, K.J. Faase, and W.H. Warnes, "Development of Multfilamentary Superconductors Containing Nb-41 WT%Ti28WT%Ta Ternary Alloys ", Adv. Cryogenic Engr., Kiuwer Academy Publisher, New York, 42:11351142 (1996). 20 M. Panek, D. Oattanayak, R. Meier-Hirner, and H. Kupfer, J. Appi. Phys., 54(12), (December):7083-7088 (1983). 21 R. Taillard, E. Florianova, C. E. Bruzek, and G. K. Hoang, Adv. Cryogenic Engr., 42:1151-1158 (1996). 22 G. K. Hoang, C. E. Bruzek, L.Oberli, and D. Leroy, 1995, IEEE Trans. Appl. Superconductivity, 5(2), (June):4 12-415 (1995). 23 P. J. Lee, J. C. McKinnell, and D.C. Larbalestier, Adv. Cryogenic Engr., Kluwer Academy Publisher, New York, 38:691-697 (1992). 24 P. J. Lee, C.M. Fischer, D.C. Larbalestier, M.T. Naus, A. A. Squitieri, W. L. Starch, R. J. Werner, P.J. Limon, G. Sabbi, A. Zlobin, E. Grogory, IEEE Trans. Appl. Superconductivity, 9(2): 1571-1574 (1999). 25 P. J. Lee, D.C. Larbalestier, J. C. Mckinnell, and A. D. Mclnturff, IEEE Trans. Appl. Superconductivity, 3(1), (March): 1354-1357 26 D. B. Chernov, et al., Titanium and Titanium Alloys. Plenum AIME. New York 2:1307 (1976). 27 T. Sasaki, K. Noto, and Y. Muto, Jap. J. Appl. Phys., 24(6):679-681(1985). 28 H. Wada and K. Tachikawa, T. Kato, IEEE Trans. Magn., MAG-17 (l):61-64 (1981). 29 M. Wake, T. Shintomi, M. Kobayashi, K. Tsuchiya, H. Hirabayashi, H. Wada, K. Inoue, K. Itoh, K. Tachikawa, K. Ishibashi, and A. D. Mclnturff, IEEE Trans. Magnetics, MAG-19 (3), (May):552-555 (1983). 30 M. Suenaga and K. M. Ralls, J. Appl. Phys., 40 (11), (October):4457-4463 (1969). 31 D. G. Hawksworth and D.C. Larbalestier, IEEE Trans. Magn., MAG-17 (1):49-52 (1981). 32 D. G. Hawksworth and D.C. Larbalestier, Adv. Cryogenic Engr., Kiuwer Academy Publisher, New York, 26:479-486 (1980). 33 N. Zhou, X. Z. Wu, Y. P. Li, Y.C. Yie, and L. Zhou, 1988, Adv. Cryogenic Engr., Kiuwer Academy Publisher, New York,., 34:995-999 (1988). 34 L.V. Potanina, G. P. Vedernikov, V. Yu. Korpusov, A.D. Nikulin, S. I. Novikov, and M. S. Novikov, Adv. Cryogenic Engr., Kluwer Academy Publisher, New York, (Materials), 44:881-887 (1998). 35 G. P. Vedernikov, L.V. Potanina, V. Yu. Korpusov, V.A. Drobishev, V.S. Zurabov, A.S. Zolotarjev, A.D. Nikulin, N.J. Kozienkova, and S. I. Novikov, IEEE Trans. Appi. Superconductivity, 7(2), (June): 1751-1754 (1997). 36 H. R. Segal, T. A. de Winter, Z. J. J. Stekly, and K. Hemachalam, IEEE Trans. Magn, MAG-17 (1), (January):53-56 (1981). 37 D.C. Larbalestier, Superconductor Materials Science, Plenum Press, New York and London (1981). 38 J. C. McKinnell, P.J. Lee, R. Resmbottom, D.C. Larbalastier, P. M. O'Larey, and W.K. McDonald, Adv. Cryogenic Engr., Kiuwer Academy Publisher, New York,34:1001-1007 (1988). 39 H. R. Segal, Z. J. J. Stekly, and A. de Winter, IEEE Trans. Magn., Mag-17 (5), (September):1645-1648 (1981). 40 D.C. Larbalestier, Adv. Cryogenic Engr., 26:10-36 (1980). 41 Liu H. and E. Gregory, 1992, IEEE Trans. Appl. Superconductivity, 3(1):13501353 (1992). 42 E. Gregory and T. Pyon, IEEE Trans. Appl. Superconductivity, 9(2): 1567-1570 (1999). 43 T. Shimada, K. Wada, S. Meguro, S. Murase, S. Nakayama, T. Orikasa, K. Makishima, K. Watanabe, K. Tsuchiya, A. Yamamoto, T. Nakamoto, and T. P. Shintomi, IEEE Trans. Appl. Superconductivity, 9(2): 1731-1734 (1999). 44 L.V. Potanina, G. P. Vedemikov, A. K. Shikov, V. Yu. Korpusov, S. V. Scherbakov, S. I. Novikov, M. S. Novikov, Adv. Cryogenic Engr., Kiuwer Academy Publisher, New York, 46(B):939 (2000) 45 L. Na and W. H. Warnes, IEEE Trans. Appi. Supercond., 1 1(1):3800-3803, (March 2001). 46 Ansel, I. Thibon, M. Bolivean and J. Debuigne, Acta metall. 46(2) (1998) 423430 47 G. Rajesh and S. V. Varamban, CALPHAD, 21(4):509-519 (1997). 48 I. Ansara, Alloy Phase Diagrams, 19:107-114 (1983). 50 APPENDICES 51 Appendix I XRD Analysis Routine If a sample contains n-phases, the intensity I, diffracted by the ith phase is proportional to the quantity of that phase present in the alloy. Intensity of the diffracted beam from a single phase powder specimen containing randomly oriented grains in the form of a flat plate in a diffractometer was first worked out by J. J. Thomson and modified later as follows: IAAf 2 I) [32 P.200Jje 2M [1 1.l(i'fF2 (1 + cos2 20 (Ito') m2jv2 k Equation Al I: integrated intensity of diffraction peak I: incident beam intensity A: incident beam cross section area X: incident beam wavelength r: radius of the diffractometer circle I..t: constant, 4ic x iO m kg C2 e: electron charge m: electron mass v: unit-cell volume F: structure factor P: multiplicity factor 0: Bragg angle e2M: temperature factor Ji: linear absorption coefficient Rewrite equation Al as: I = KR Equation A2 2Paiioy where: = +W2 W1 I PJi P)aiioy r 2 K=b0A2hb0 32,rr + [P1 LLJ e1 Tj Equation A3 52 ±JF2P(1 + cos2 20 J]e2M sin2Ocos9 R v[ K is the first two terms of equation Al, and is independent of diffraction materials, and therefore being considered as a constant. R is combination of the third, the fourth and the fifth terms of the equation Al. R, depends on the nature of the phase, diffraction angle (0) and hkl. Notice that the equation Al is true only for the single-phase alloy. When calculating an intensity of reflection from one phase out of a mixture of phases, we multiply the right hand side of equation Al by Ca, the volume fraction of the a-phase in the alloy. Manipulating Equation Al, A2 and taking account of the volume fraction factor Ca the intensity of a reflection of the a-phase can then be written as KRC Equation A4.l 2/'a!loV KRC 2 ,8 fi Equation A4.2 alloy So, the volume fraction ratio of two phases is: C RI fi a Cf3 RaIp Equation AS. Ca+C1 Equation A5.2 R can be worked out from XRD results, described in details in the follows. Combining equation A5. 1 Determination and A5.2, the volume fraction of each phase can be obtained. of R value: In order to know the proportion of each phase, we need to know the integrated intensity ratio of the two phases and the R ratio of the two phases. The integrated intensities are obtained from the XRD experiment. R-values are obtained from the following procedures. 1 53 Fp 7 R ( V ) l+cos22OB S111OBCOSOB J] Here we ignore the temperature effect because all we run is in a constant (room temperature) condition. v = a3 for BCC V = 0.866 a2 c for Hexagonal Multiplicity Factor (P) Table Al Multiplicity factors HCP (alpha-Ti) 16] BCC (beta-Nb,Ta) hkl P hid P 002 6 110 12 101 12 200 6 102 12 211 24 103 12 220 12 Lorentz-Polarization Factor (LPF) The overall effect of this geometrical factor is to decrease the intensity of reflection of 0, and is described as: 1+ cos2 20 sin2 Ocos 0 Structure Factor B CC: F = f e2°+f e2 2+d22)=f F=2f, h+k+l = even; F = 0, h+k+1 = odd. HCP: F= f [l+e223'2J; [1 +e] 54 Atomic Scattering Factor (ASF) ASF is used to describe the "efficiency" of scattering of a given atom in a given direction. The atomic scattering factor data was taken from reference6, and then plotted in Excel. The best fit is derived from the plot and shown in the following equations. ASFT=21 .03-18.8 15x- 142.06x2+538.41x3-796.3 1x4+541 .25x5- 139.53x6 ASFNh=4 1.041-1 6.559x-295.74x2+972.9x3- 1 348.4x4+876.99x5-2 1 8.65x6 ASFT=73.017-24.878X-379.19X2+1094 1x3-1349x4+789.21x5-178.66x6 ASF=56.055-20.496x-334.96x2-i- 1029.9x3- 1 348.7x4+835.73x5- 1 99.86x6 Here, x=SinO/X. 80 70 0 0 U- C 0 4- 30 0 0.2 0.4 0.6 0.8 1 1.2 1.4 Sin/Iamda Figure Al. The atomic scattering factors. "% of beta" is taken from wt % of niobium and wt % tantalum. Nb24Ta49Ti is shown here. However, the difference between the average value and percentage value is small. In this writing, average value is used for all ternary samples. 55 Appendix II. Regular Solution Models of Ternary Phase Equilibria Ternary Phase: This appendix contains derivation of regular solution models based on the model of Kaufman's F This model has been applied explicitly in terms of the pairwise interaction parameters determined numerically. MATHEMATICA has been used to solve the equation systems for equilibrium between the solution phases (a and 1). The governing equation is shown as: Fa[xa,xfl ...x" ,T] = x1 F10[T]TAS + i=1 Equation A6 i=1 j=i xi = 1 AS = R Equation A6. 1 ln Notations are listed in Table A2. Where: is the atomic fraction of element i, T is the absolute temperature in Kelvin, F1a [T] is the free energy of pure element i in a phase, and Ea is the a structure interaction parameter between elements i and j. This equation is the extension of the regular solution model which has been applied to binary systems in equation 4. The equilibration of the partial free energies of i, j, and k across the two-phase region, as shown in Figure A2 is: -a -fl F (x,y)_Fi (xp,yfl) -a -/j F (x,y) = F (xp,yp) -a -fl Fk(x,y) = Fk (xfl,yfl) Equation A7 56 Where the partial molar free energies of i, j, k in the c and 3 phases are given by: F F° x dx y dy =F' F = F° +y2E +xyAEa aF (lx) 9Fdx ay Fe +RTlnx+(l x)2E1 + y2 aFa F = F° +(ly) c?x dy +(l x)yAEa Equation A8 x = Fk0 +RTlny+x2 +(1y)2E1 x(ly)zE AEa =E+EE The other partial free energies are defined similarly. Combining equation A6, A7 and A8 yields three equations relating xa, y, x, y, and T: +Rfln(Z±)+(E4 F4x)+(Ey Ey)+(AExflyfl F' F =AF Za x8 F_Ff =A+RTln(--)+(E(lxfl)2E(lxa)2)+(EyE,y) Xcx (AE(l--x)y F Fj =z' =0 +Rfln(2)+(Ex2 _4x2)+(E(1_yp)2 E1(1y)2 Ya (LE(1yfl)x =0 Equation A9 Table A2. The notations used in NbTiTa ternary system Niobium Titanium Tantalum At. % of elements Z Y X Elements I K J 57 f common tonqency Locus of poafs \\ ji F{*yT] iii I I H I I liwo pho4e region i I I I / /1 / Pose 7jii III I PPase ''ii 'I I / / trie -_-L K I F1x.yo]1 ii I --t-- ,y.} I I ty) Figure A2. Free energy representaion of the formation of ternary-solution phase equilibria. The phase diagram projected below results from the interaction of free energy surface as shown'11. Binary Phase: For binary system, the equation A6 reduced to: F[xl1,xfl,T] = (i x)Fx+ xF1'+ RT[xlnx+(1 x)ln(1 x)]+ cal/g-atom Equation AlO is the excess free energy of the mixing which is zero when x=O and 1. In regular solution model, the excess free energy is given by =B x (1-x) cal/g atom where: B is the interaction parameter and B=O for ideal solution. The partial free energy of components i and j is: F = F" i-'a x dx F =F"(lx) Equation Al 1 d F" dx Notice that the equation Al 1 is reduced from equation A8. Now, we take partial derivatives respect to the x according to equation A 10: -- F" +(1x) dx +F'+x 9x +B(lx)Bx+RT[lnx+1---ln(1x)-1] F" + F" + B 2Bx+RT[lnxln(1x)} Equation Al2 Insert equation AlO and Al2 into All, we have: (lx)F"+xF1"+RT[xlnx+(lx)1n(lx)]+Bx(1x) {_i" +F" +B-2Bx+RT[lnxln(1x)1} = = F" + RT1n(1 x) + Bx2 Equation A14 Similarly, Fi" = FJ" +RTlnx+B(lx)2 Equation A15 x is at % of element of j. Similar expression can be obtained for phase. 1 Equation A16 7=F/3 +RT1n(lx)+Bx2 Ff = Ff +RTlnx+B(1x)2 EquationAl7 Applying the equilibrium conditions: a' =F/fl a' flj =F1 F1 xa P Equation Al8 xIJ Combination of equation Al4-A18 yields F1" F= RT1n(1 X lxflJ B(x) 2 A(xa2 ) Equation A19 F1 Ff = = RTln[J+ B(l x)2 A(1f)2 Equation A20 where: A and B are the regular solution interaction parameters for the hcp and bcc phase in i-j systems. Simultaneous solution of A19 and A20 yields the equilibrium composition of the a and J3 phases. Appendix III Critical Temperature Measurement The data acquisition software adjusts the temperature set points, waits for stable temperature, and then records the lock-in amplifier output. The data pair of lock-in output and temperature is recorded and a new temperature set point is determined. Thus, the change in magnetic susceptibility of the sample is recorded, as shown in Figure a. The starting point of the Tc transition in each of two witness coils and the on-site liquidhelium-temperature are recorded as the critical temperatures of pure niobium, pure lead, and liquid helium. These three points with ideal critical temperatures of these three points (Tc(NB)= 9.3, Tc(PB)= 7.2, TC(OK)= 4.2) are plotted, and fitted with quadratic function, as shown in Figure b. According to this quadratic fit function, the Tc data is replotted with calibration data points, as shown in Figure c. Then, a corrected critical temperature of the sample is determined from the 10%, 50% and 90% transition height data. 50% of Tc is reported as our critical temperature. 61 Figure A3. Critical Temperature Measurement Nb49Ti24Ta-400C- 1 000H (AC corrected) E EfE L14i: 1.50E-05 0QOOQC) 000000000000000000000000 0 a a'o 000 IXIOD Nb49Ti24Ta-400C- 1 000H L. IUL)O 1.90E-05 . L7OE-05 150E-05 L3OE-05 1.10 E-05 9.00EOo - 7.00E06 c mn C' C' r 0 U) C' C' C' U) 0 C' r'. o o o$ 0 U) C' C' 0 0 C' - , Temperature(K) WAC 2449-400C- 1 000H Temperature Calibration 10.00 2i,7xo4o39 TH01T5T : 4.00 5.00 6.00 7.00 WAC Points (K) 8.00 9.00 10.00 62 Appendix IV-Critical Temperature Data Figure A4. The Critical Temperature Verses the Heat Treatment Tc versus Treatment: Nb46TI 1 2Ta 11 ': 8 - Il2hrs. 7 2 6 I(1 - 5 50% 4 Trnsidon Width Nb46Til2Ta-AR Nb46TjI2Ta-41J01000 Nb46Ti I2Ta-450-300 Nb46Ti l2Ta-500-300 Nb46Til2Ta-550-600 Nb46TiI2Ta-600-600 Treatment Ic versus Trealment: Nb3911 1 81a 5 50% Ic 4 lsitionWiihh 3 2 Nb39Til8Ta-AR Nb391j1 8Ta-4001000 Nb39Ti l8Ta-450-300 Nb39Til 8Ta-500-300 Nb39Til8Ta-550-600 Nb39Til8Ta-600-600 Treatment 63 Figure A4. The Critical Temperature Verses the Heat Treatment-Continued Ic versus Treatment: Nb5lTil5Ta 11 fl2h 5O%Tt 4 Transithn Width 3 2 112 hp 1 0 Nb5 lTil5Ta-AR Nb5lTi l5Ta-400- Nb5 lTjl5Ta-450-300 Nb5 lTil5Ta-500-300 Nb5 iTi l5Ta-550-600 Nb5lTi lSTa-600-600 1000 Treatment Ic versus Treatment: Nb49T124Ta 8 2 4 T1S11iOR Width 3 2 H2hrs. 1 0 Nb49Ti24Ta-AR Nb49Ti24Ta-400- Nb49Ti24Ta-450-300 Nh49Ti24Ta-500-300 Nb49Ti24Ta-550-600 1000 Treatment Figure A4. The Critical Temperature Verses the Heat Treatment-Continued Tc versus Treatment: Nb41 Ti28Ta 11 ':: 8 7 2 6 - 5---- IC) 3-- - 50%lb TnSton Width 2 112 h. I 0 Nb4ITI28Ta-AR . Nb4ITj28Ta-450-300 Nb4ITi28Ta-500-300 Nb4ITI28Ta-550-600 Nb4ITi28Ta-600-600 Treatment Ic versus Treatment: Nb44Ti 1 7Ta 'ItI 5O%T U Tanflo Width çTITII1_ Nb44Til7Ta-AR Nb44Til7Ta-400- Nb44Til7Ta-450-300 Nb44Til7Ta-500-300 Nb44Til7Ta-550-600 Nb44Ti-17Ta-600600 1000 Treatment 65 Figure A4. The Critical Temperature Verses the Heat Treatment-Continued Tc versus Treatment: Nb55TI Binary --*._______ 12 .._ :ii_ _ 7 6 5 50% Tc Ttaitkm Width 2 I 12 Iuc. Nb55Ti-AR Nb55Ti-450-300 Nb55Ti-500-300 Nb55Ti-550-600 Treatment Ic versus Treatment: Nb47Ti Binary E I 50% Yc 4 ThnsitotWidth1 3 ---T Nb47TI-AR Nb47Ti-400-300 Nb47Ti-450-300 Nb47Ti-500-300 Treatment Nb55Ti-600-600 Figure A4. The Critical Temperature Verses the Heat Treatment-Continued Tc versus Treatment: Ta5OTi Binary l0 9 8 7 6 4 3 0 Ta5OTi-AR TaSOTi-450-300 Ta50Ti-500300 Treatment Ta5OTi-550-600 Ta5OTi-600-600 67 Table A3. Critical Temperatures at different aging temperatures and aging times. SampleName 10%Tc 50%Tc 90%Tc ATc Nb46Til2Ta-AR 8.15 8.23 8.29 0.14 Nb5lTilSTa-AR Nb44Til7Ta-AR Nb39Til8Ta-AR 8.4 8.55 8.8 0.4 8.7 10.15 10.7 2 9.21 9.39 9.55 0.34 Nb49Ti24Ta-AR 7.5 8.75 9.52 2.02 0.04 Nb4lTi28Ta-AR 8.94 8.96 8.98 Nb47Ti-AR 8.53 9.15 9.45 0.92 Nb55Ti-AR 8.42 8.7 8.87 0.45 Ta5OTi-AR 6.13 6.65 7.22 1.09 Nb46Til2Ta-400-1000 7.39 8.74 9.43 2.04 Nb5lTiI5Ta-400-1000 Nb44Til7Ta-400-1000 8.65 8.83 9.06 0.41 8.92 9.04 9.15 0.23 Nb39Til8Ta-400-1000 8.6 8.8 9 0.4 Nb49Ti24Ta-400-1000 8.67 9.47 9.74 1.07 Nb4lTi28Ta-400 N/A N/A N/A N/A Nb47Ti-400-300 8.13 8.23 8.32 0.19 Ta5OTi-400 N/A N/A N/A N/A Nb46Til2Ta-450-300 8.35 8.95 9.2 0.85 Nb5lTil5Ta-450-300 Nb44Til7Ta-450-300 Nb39Til8Ta-450-300 9.14 9.32 9.41 0.27 9.46 9.74 9.85 0.39 9.18 9.57 9.89 0.71 Nb49Ti24Ta-450-300 9.3 9.37 9.38 0.08 Nb4lTi28Ta-450-300 9.14 9.25 9.28 0.14 Nb47Ti-450-300 8.96 8.99 9.06 0.1 Nb55Ti-450-300 10.1 10.56 10.96 0.86 Ta5OT1-450-300 7.63 7.98 8.06 0.43 Nb46Til2Ta-500-300 9.01 9.69 10.33 1.32 Nb5lTil5Ta-500-300 9.09 9.24 9.37 0.28 Nb44Til7Ta-500-300 10.03 10.19 10.23 0.2 Nb39Til8Ta-500-300 9.2 9.23 9.26 0.06 Nb49Ti24Ta-500-300 9.3 9.34 9.35 0.05 Nb4lTi28Ta-500-300 9.61 9.76 9.87 0.26 Nb47Ti-500-300 9.44 9.76 9.97 0.53 Nb55Ti-500-300H 9.29 9.31 9.32 0.03 Ta5OTi-500-300 8.41 8.59 8.7 0.29 Nb46Til2Ta-550-600 8.07 8.55 9 0.93 7.22 7.68 8.35 1.13 9.67 9.88 10.21 0.54 Nb44Til7Ta-550-600 9.1 9.56 9.95 0.85 Nb39Til8Ta-550-600 9.61 9.63 9.65 0.04 Nb49Ti24Ta-550-600 8.8 8.93 8.99 0.19 Nb4lTi2STa-550-600 9.7 9.8 9.88 0.18 Nb55Ti-550-600 8.3 8.75 8.83 0.53 Ta5OTi-550-600 7.99 8.14 8.22 0.23 Nb46Til2Ta-600-600 8.65 9.29 10.05 1.4 -550-300 Nb5lTil5Ta-550-600 LSIJ Table A3. Critical Temperatures at Different Aging Temperatures and Aging Times-Continued. Nb5lTil5Ta-600-600 Nb49Ti24Ta-600-600 Nb44Ti-l7Ta-600-600 Nb39Til8Ta-600-600 Nb4lTi28Ta-600-600 Nb55Ti-600-600 Ta50Ti600-600 9.21 9.39 9.55 0.34 6.83 '7.08 7.31 0.48 7.91 8.28 8.47 0.56 9.46 9.95 10.18 0.72 9.44 9.56 9.68 0.24 8.13 8.25 8.36 0.23 7.17 7.29 7.4 0.23 Nb46Til2Ta-500-112 7.12 8.7 9.06 1.94 Nb5lTil5Ta-500-112 Nb44Til7Ta-500-112 9.53 9.61 9.71 0.18 10.02 10.09 10.14 0.12 Nb39Til8Ta-500-112 9.54 9.6 9.71 0.17 Nb49Ti24Ta-500-1 12 9.21 9.28 9.36 0.15 Nb4lTi28Ta-500112 9.74 9.88 9.94 0.2 N/A Nb47Ti-500-112 N/A N/A N/A Nb55Ti-500-112 10.64 10.77 11.08 0.44 Pure NB sheet 8.91 9.00 9.08 0.17